This lecture outlines the metallurgical principles of alloy selection and specifications. Basic knowledge of physics and chemistry and some familiarity with TALAT lectures 1201 through 1205 is assumed.
TALAT Lecture 1255: Metallurgical Background to Alloy Selection and Specifications for Wrought, Cast and Special Applications
TALAT Lecture 1255
Metallurgical Background to Alloy Selection and
Specifications for Wrought, Cast and Special
16 pages, 17 Figures
Advanced level I
prepared by M H Jacobs
Interdisciplinary Research Centre in Materials
The University of Birmingham, UK
Outline of the metallurgical principles of alloy selection and specifications.
Basic knowledge of physics and chemistry. Familiarity with the contents of Lectures
1201 through 1205.
Date of Issue: 1999
EAA - European Aluminium Association
1255 Metallurgical Background to Alloy Selection
and Specifications for Wrought, Cast and
Contents (17 Figures)
1255 Metallurgical Background to Alloy Selection and Specifications for
Wrought, Cast and Special Applications ___________________________________2
1255.01 Wrought alloys____________________________________________________ 3
1255.01.01 Designation of wrought alloys _________________________________________3
1255.01.02 Wrought alloy selection ______________________________________________5
1255.02 Cast alloys________________________________________________________ 7
1255.03 Aerospace alloys___________________________________________________ 9
1255.03.01 Fine tuning of established alloys_______________________________________10
1255.03.02 Aluminium-Lithium based alloys ______________________________________11
1255.04 Novel processing and special alloys __________________________________ 12
1255.04.01 Hot Isostatic Processing of Aluminium Castings __________________________12
1255.04.02 Particulate processing _______________________________________________13
1255.04.03 Particulate Metal Matrix Composites ___________________________________14
1255.04.04 Rapid solidification processing (RSP) __________________________________15
1255.05 References_______________________________________________________ 16
1255.06 List of Figures ___________________________________________________ 16
TALAT 1255 2
1255.01 Wrought alloys
The majority of aluminium used in engineering applications is in the wrought form
; that is, as rolled plate, sheet and foil, extrusions, tube, bar and wire (the remainder
are casting alloys and alloys produced by special processing - we will consider these
later in this TALAT lecture).
The number of alloys available to the engineer is large, but can be divided into two
main groups; non-heat treatable alloys and heat treatable alloys. Before looking at
the characteristics of these two classes of wrought alloy, let us first define the modern
method of designation of wrought alloys and their processing.
1255.01.01 Designation of wrought alloys
The International Designation System for wrought alloys is reproduced below in
Table 1 and also in Figure 1255.01.01.
AA Designation Major alloying elements
1xxx None ) Non - heat treatable
3xxx Mn )
4xxx Si ) Non - heat treatable
5xxx Mg )
2xxx Cu )
6xxx Mg + Si ) Heat treatable
7xxx Zn )
8xxx Other )
Table 1. Designation of wrought aluminium alloys.
In this four digit classification system, the first digit identifies the major alloying
elements(s). The remaining three digits are used as serial numbers to identify
particular alloy types. For the 1xxx series there is some logic in the designations; for
example, in alloys of commercial purity, the xxx signifies the degree of purity - 1080
signifies aluminium of purity 99.80 wt%. For the remaining wrought alloys the xxx
in the designation has no systematic code and the reader is referred to texts such as
that provided by the Aluminium Federation .
TALAT 1255 3
The processing condition of an aluminium alloy is given by its temper designation,
which is a convention for describing the basic treatment or condition of the alloy
(Note : here the term ‘temper’ has a different meaning to the very specific heat
treatment of ‘tempering’ as applied to steels).
Temper designations for aluminium alloys as per the American Aluminium
Association are given in Figure 1255.01.02. Unfortunately, variations of this
classification persist in the UK and Europe (see  and ).
TALAT 1255 4
1255.01.02 Wrought alloy selection
Wrought aluminium alloys are selected, Figure 1255.01.03 on the basis of
- the properties required during service;
- the ease of forming and fabrication;
- and last but not least, the overall cost of alloy type, availability, heat treatment
processing and finishing.
The alloys may be divided into two groups, non-heat treatable alloys and heat
treatable alloys, Figure 1255.01.04.
TALAT 1255 5
1255.01.02.01 Non-heat treatable alloys
These alloys, Figure 1255.01.05, are hardened by solution hardening and/or by work
hardening, but they do not respond to heat treatment by precipitation hardening.
Pure aluminium (1xxx series) finds applications in electrical conductors, certain plant
for chemical engineering and for architectural panels. Tensile properties are low in the
annealed condition (~ 50MPa) and can be doubled by cold work.
Alloys selected from the 3xxx series alloys, based on Al-Mn , such as 3003, are used
as sheet material, for example for aluminium car radiator corrugations. They are used
in applications which require medium strength (~ 180 MPa) together with good
ductility (i.e. ease of forming) and good corrosion resistance. For example, 3004, with
Mn and Mg, for beverage cans .
Alloys from the 5xxx series, based on Al-Mg, are used  as structural plate for
transport applications, and with alloys made from high-purity aluminium may be
polished to a bright finish for automotive trim and architectural panels.
1255.01.02.02 Heat treatable alloys
The alloy series are 2xxx, 6xxx, 7xxx and 8xxx, so the choice for selection is large.
All depend upon precipitation hardening in order to develop their optimum properties,
The 2xxx series, particularly those based on Al-Cu-Mg have found application in
aircraft structures .
Al-Mg-Si alloys (6xxx) series are used extensively as medium strength extrusions
with a wide field of application.
TALAT 1255 6
he Al-Zn-Mg alloys (7xxx series) offer high strength  for demanding applications.
Special heat treatable alloys in the 8xxx series include 8001 (Al-1.1Ni-0.6Fe) for
nuclear plant  where it resists corrosion in water at high temperatures and
pressures, and 8011 (Al-0.75Fe-0.7Si) with excellent deep drawing properties for
bottle tops .
1255.02 Cast alloys
Designations of casting alloys as classified by the American Aluminium Association
are given in Figure 1255.02.01 and Table 2.
TALAT 1255 7
The use of other designations is common-place, for example the LM series in the UK
- see  and .
As with wrought alloys, casting alloys may also be divided into those with are non-
heat treatable and those which are heat treatable.
Selection of casting alloys, Figure 1255.02.02 depends upon the type of casting
process and the properties required by the application, see TALAT lecture 3201,
Introduction to Casting Technology.
AA Designation Major alloying elements
1xx.x None )
4xx.x Si ) Non - heat treatable
5xx.x Mg )
2xx.x Cu )
3xx.x Si + Cu / Mg )
7xx.x Zn ) Heat treatable
8xx.x Sn )
9xx.x Other )
Table 2. Designation of casting aluminium alloys.
Casting aluminium alloys based on those to which silicon is added as the main
alloying element are probably the most important for engineering applications. This is
because of the high fluidity provided by alloys with near eutectic composition. The
castings have high corrosion resistance, combined with a low coefficient of thermal
expansion and good weldability .
TALAT 1255 8
1255.03 Aerospace alloys
An excellent summary of the essential role of aluminium alloys in the aerospace
industry is presented in the Aluminium File . The special demands of civil and
military air travel have placed the aerospace industry at the forefront of the
technologies of lightweight materials, and aluminium alloys have an important role in
this field of high performance application. In  it is said that “high strength
combined with aluminium’s low density offers obvious advantages to other uses but
factors such as toughness, fatigue performance and sensitivity to environmental
effects must be taken into account when considering aircraft alloys for applications
which differ from their original purpose. Of prime importance is the need for
minimum weight consistent with safety, initial fabrication costs plus cost of
ownership for the required service life”.
Aluminium alloys are used for many aerospace applications, mainly for the airframe
structure, including the skin material. Again as reported in , “airframes are subject
to combinations of both static and dynamic stresses depending on the part in question
and they operate in a range of internal and external environments. They are subject to
temperature changes caused by the atmosphere and speed. Also, should any defect
occur during flight, the material used must be capable of tolerating its effect until the
fault can be detected and identified at inspection. Furthermore, the demands of such
damage tolerance vary depending on the component in question. Consequently, the
additional material properties to be adjusted around the required mechanical
properties, or perhaps vice versa, are fatigue, stress corrosion, pitting corrosion,
exfoliation corrosion, galvanic corrosion, fracture toughness and the effects of
temperature. Also, fabrication factors - machining, forming and joining - have to be
taken into account” - Figure 1255.03.01. Also, it must be emphasised that the
aerospace industry, quite rightly for our safety, requires any new material or new
variant of a material to be thoroughly tested, proven and certified before it is ever
considered for service. This means that the lead times before the introduction of any
new material are necessarily long.
TALAT 1255 9
The aluminium industry has responded to these demands in three ways,
Figure 1255.03.02: firstly, by ‘fine tuning’ existing alloys to provide the performance
characteristics required for specific applications; secondly, by development of new
alloys - for example, those which contain Lithium for further weight reduction and
improved specific stiffness; and thirdly, by developing special alloys by novel
processing techniques. The first two approaches are described in the remainder of this
chapter, the third on the production and application of special alloys by novel
processing is given its own section below - because it has wider application than just
1255.03.01 Fine tuning of established alloys
It should be noted that aircraft development during World War 2 stimulated the
introduction of high strength 7xxx series aluminium alloys based on Al-Zn-Mg-Cu,
with tensile strengths exceeding 500MPa.
Since that time , further developments of the 7xxx alloys for strength-critical areas,
and development of the 2xxx series alloys for damage-critical areas, have taken place,
In the case of the 7xxx developments, these have been concentrated  on improving
service reliability by enhancement of resistance to stress-corrosion cracking and
fracture toughness via fine tuning of heat treatment and small changes to alloy
composition rather than any major improvement in tensile strength. This has been
achieved  by the optimisation of two-step ageing treatments (see TALAT
Lecture 1204), in some cases by combining ageing with deformation to achieve a
measure of strengthening from dislocation hardening. Commercial considerations
have restricted disclosure of the details of such processing, but it is interesting to note
that it is reported  that a 7055 alloy (Al-8Zn-2.05Mg-2.3Cu-0.16Zn-0.15Femax-
TALAT 1255 10
0.10Simax) has been used for structural members of the Boeing 777 giving a weight
saving ~ 635kg.
2xxx series alloys continue to be used as aircraft structural materials, for example as
fuselage skins. Enhanced fracture toughness has been achieved by improvements in
alloy cleanness, for example, lower levels of iron and silicon. Alloy 2618 (Al-2.2Cu-
1.5Mg-1Ni-1Fe) is used as the fuselage skin of Concorde, with the Cu and Mg
providing precipitation hardening and FeNiAl9 dispersoid particles stabilising the
1255.03.02 Aluminium-Lithium based alloys
The addition of lithium to aluminium alloys both reduces weight (density is reduced
by 3% for each 1%Li added) and increases the stiffness (the elastic modulus is
increased by 6% for each 1% Li added , Figure 1255.03.04. This attractive
combination of enhanced properties has stimulated much research into these alloys,
and this continues. Low fracture toughness has been a problem, attributed to grain
boundary segregation of sodium and potassium - measures have been taken to clean
melt alloys to achieve material with less than 1 ppm of Na and K impurity levels .
TALAT 1255 11
1255.04 Novel processing and special alloys
Following the revolution in scientific understanding of the metallurgy of aluminium
alloys in the 1960s that occurred as a result of the application of the transmission
electron microscope to the investigation of microstructure, there was a period of
consolidation and optimisation that led to the family of alloys that we know today. It
is not unreasonable to say that the bounds of metallurgy imposed by equilibrium
phase diagrams have been thoroughly explored. This should not imply that there will
always be scope for ‘fine tuning’, as we have seen for aerospace alloys above. Maybe
a similar ‘fine tuning’ will be promoted by the drive towards the aluminium
automobile. None the less, the bounds of equilibrium metallurgy will only be
stretched so far, and this has been recognised over the last four decades. However, we
have not reached the end of the road; new processes have been, or are being,
developed either to compensate for the limitations imposed by ‘equilibrium
metallurgy’ or to exploit ‘non-equilibrium’ processes. In this section we will look at
examples of technologies in these categories.
1255.04.01 Hot Isostatic Processing of Aluminium Castings
Hot isostatic pressing (HIPping) involves  the application to a component of
processing conditions of elevated temperature and a very high gas pressure, say
~ 100MPa (about 1000 bar or atmospheres) in a special hot isostatic processing plant,
Figure 1255.04.01. Thus, a very high isostatic gas pressure is applied to the
component to be treated which, provided the temperature is high enough for plastic
deformation and creep to occur, will consolidate with any pores being closed.
HIP processing is applied to aluminium castings, commonly at ~ 500°C for a few
minutes at a gas pressure ~ 100MPa. Shrinkage porosity is closed, but the as-cast
microstructure is not significantly changed. The beneficial reason for HIPping is that
TALAT 1255 12
the ultimate tensile strength of a casting may be increased by 10-20%, and the
ductility may be doubled .
Hence, HIPping may be seen as a method of counteracting the natural interdendritic
porosity that occurs during solidification of an aluminium casting.
Very large HIPping plant is now in commercial operation , which reduces the unit
cost to a level which makes it a worthwhile for the enhanced mechanical properties
It must be pointed out however, that HIPping must not be seen as a way of correcting
bad casting practice. Currently, computer modelling is very successfully being
applied to the design of casting systems in order to obtain the highest integrity of cast
product. Also, the avoidance of trapped, folded oxide films is paramount , which
again comes down to devising good casting practice.
1255.04.02 Particulate processing
Aluminium alloys may be processed to prepare powder and sprayformed products by
gas atomisation, Figure 1255.04.02, and by centrifugal atomisation,
Atomisation caused rapid solidification, and this may be usefully employed to
increase the amount of solute retained in solid solution; for example, alloys with high
lithium contents up to ~ 5% may be made in this way.
The injection of oxide or carbide powder into a sprayformed product is one method of
manufacturing a metal matrix composite (MMC). Other methods of making MMCs
include infiltration of a porous ceramic with molten aluminium and stirring of
particulates into molten aluminium.
TALAT 1255 13
1255.04.03 Particulate Metal Matrix Composites
Special attention has been paid  to composites of aluminium alloys such as 2014
(Al-Cu-Mg-Mn) and 6061 (Al-Mg-Si) with silicon carbide or alumina particles or
fibres, Figure 1255.04.04. 6061-SiC MMCs have been developed as extrusions with
up to 20 volume % SiC as short fibres; this gives high tensile strength (~500MPa) and
a high elastic modulus at 120GPa compared with 70GPa for 6061.
TALAT 1255 14
1255.04.04 Rapid solidification processing (RSP)
Rapid solidification may be achieved by atomisation or injection of a molten stream
of aluminium alloy on to a cold rotating disc, Figure 1255.04.05. Cooling rates are
the order of 106°C s-1.
Al-Fe with Fe contents around 8% are commonly used as the base for RSP aluminium
alloys. Fe has virtually no equilibrium solubility in Al, see TALAT lecture 1203 and
Figure 1203.01.09. However, by very rapid solidification the Fe may be forced into
high metastable solid solution, which then precipitates fine-scale metastable phases
which confer useful mechanical properties on the alloy - particularly higher strength
at elevated temperatures of around 300°C to 400°C .
TALAT 1255 15
1. I J Polmear, Light Alloys : Metallurgy of the Light Metals, Edward Arnold, 1989.
2. Aluminium Federation, The Properties of Aluminium and Its Alloys, ALFED UK,
3. E C Rollason, Metallurgy for Engineers, Edward Arnold, 1958.
4. The Aluminium File. Part 8.3 : Case Histories - Aerospace Applications, The
Aluminium Federation, UK, 1997.
5. I J Polmear, Recent Developments in Light Alloys, Materials Transactions, JIM,
Vol 37, No 1, pp 12-31, 1996.
6. H V Atkinson and B A Rickinson, Hot Isostatic Processing, The Adam Hilger
Series on New Materials. Series Editor J Woods, 1991.
7. J Campbell, Castings, Butterworth Heinemann, 1991.
1255.06 List of Figures
Figure No. Figure Title (Overhead)
1255.01.01 Classifications of Aluminium Alloys
1255.01.02 Temper designations
1255.01.03 Factors for wrought alloy selection (Wrought alloy selection /1)
1255.01.04 Wrought alloy selection /2
1255.01.05 Examples of non-heat treatable alloys (Wrought alloy selection /3)
1255.01.06 Examples of heat treatable alloys (Wrought alloy selection /4)
1255.02.01 Designation of casting alloys
1255.02.02 Selection of casting alloys
1255.03.01 Factors in selection of aerospace aluminium alloy
(Aerospace alloys /1)
1255.03.02 Development of aerospace aluminium alloy (Aerospace alloys /2)
1255.03.03 ‘Fine tune’ established alloys (Aerospace alloys /3)
1255.03.04 Al-Li based alloys (Aerospace alloys /4)
1255.04.01 Hot Isostatic Processing (HIPping) of Aluminium castings
(Novel processing /1)
1255.04.02 Particulate Processing of Aluminium (Novel processing /2)
1255.04.03 Centrifugal atomisation (Novel processing /3)
1255.04.04 Metal Matrix composites (MMCs) (Novel processing /4)
1255.04.05 Rapid Solidification Processing (RSP) (Novel processing /5)
TALAT 1255 16